Effect of iron on the microstructure and mechanical property
of Al–Mg–Si–Mn and Al–Mg–Si diecast alloys
, Wenchao Yang, Feng Gao, Douglas Watson, Zhongyun FanBrunel Centre for Advanced Solidiﬁcation Technology (BCAST), Brunel University, Uxbridge, Middlesex, UB8 3PH, UK
a r t i c l e
i n f o
Received 30 July 2012 Received in revised form 20 October 2012
Accepted 26 November 2012 Available online 1 December 2012
Aluminium alloy Mechanical properties Fe-rich compounds High pressure die casting CALPHAD
a b s t r a c t
Al–Mg–Si based alloys can provide super ductility to satisfy the demands of thin wall castings in the application of automotive structure. In this work, the effect of iron on the microstructure and mechanical properties of the Al–Mg–Si diecast alloys with different Mn concentrations is investigated. The CALPHAD (acronym of Calculation of Phase Diagrams) modelling with the thermodynamic properties of the multi-component Al–Mg–Si–Mn–Fe and Al–Mg–Si–Fe systems is carried out to understand the role of alloying on the formation of different primary Fe-rich intermetallic compounds. The results showed that the Fe-rich intermetallic phases precipitate in two solidiﬁcation stages in the high pressure die casting process: one is in the shot sleeve and the other is in the die cavity, resulting in the different morphologies and sizes. In the Al–Mg–Si–Mn alloys, the Fe-rich intermetallic phase formed in the shot sleeve exhibited coarse compact morphology and those formed in the die cavity were ﬁne compact particles. Although with different morphologies, the compact intermetallics were identiﬁed as the samea-AlFeMnSi phase with typical composition of Al24(Fe,Mn)6Si2. With increased Fe
content,b-AlFe was found in the microstructure with a long needle-shaped morphology, which was identiﬁed as Al13(Fe,Mn)4Si0.25. In the Al–Mg–Si alloy, the identiﬁed Fe-rich intermetallics included the
compacta-AlFeSi phase with typical composition of Al8Fe2Si and the needle-shapedb-AlFe phase with
typical composition of Al13Fe4. Generally, the existence of iron in the alloy slightly increases the yield
strength, but signiﬁcantly reduces the elongation. The ultimate tensile strength maintains at similar levels when Fe contents is less than 0.5 wt%, but decreases signiﬁcantly with the further increased Fe concentration in the alloys. CALPHAD modelling shows that the addition of Mn enlarges the Fe tolerance for the formation ofa-AlFeMnSi intermetallics and suppresses the formation ofb-AlFe phase in the Al–Mg–Si alloys, and thus improves their mechanical properties.
&2012 Elsevier B.V. All rights reserved.
In Al–Mg–Si based alloys that can provide super ductility in castings , iron is a common impurity element but it is unavoidably picked up during melting and casting, and particu-larly when the scraped and recycled materials are used. Although the presence of iron is beneﬁcial to prevent die soldering in high pressure die casting (HPDC) process[2,3], the excessive iron has been found to be detrimental to the mechanical properties of Al–Si, Al–Si–Cu and Al–Si–Mg alloys[4,5]. Generally, the effect of Fe-rich phases on the mechanical properties of aluminium alloys depends on their type, size and amount in the microstructure.
A variety of Fe-rich intermetallic phases have been observed in aluminium alloys. In Al–Si–Fe system there are ﬁve main Fe-rich phases: Al3Fe (or Al13Fe4),
g-Al3FeSi[6,7]. Among them,
b-Al5FeSi usually appears as highly faceted platelets up to several milli-metres and it therefore causes the most serious loss of strength and ductility in the castings[8,9]. However, the
a-Al8Fe2Si phase has been reported as the compounds with many different types of morphology [10,11]. The morphological changes from plate to Chinese script or compact shapes were reported to enhance mechanical properties [12,13]. On the other hand, manganese has been widely used to suppress the development of long needle-shaped Fe-rich phases and to promote the formation of compact Fe-rich phases in aluminium alloys. In hypoeutectic Al–Si alloys containing Fe, Mn and Mg, three Fe-rich phases of
p-Al8FeMg3Si6compounds have been identiﬁed [8,15]. In the commonly used Al–Si–Mg cast alloys, with a Mn/Fe ratio of 0.5, the structure of Fe-rich inter-metallics is body centred cubic
a-Al15(FeMn)3Si2 [16,17], which may appear as hexagonal, star-like, or dendritic crystals at different Mn/Fe ratios. However, in the various results from previous studies, the effect of Fe on the microstructure is in good
Contents lists available atSciVerse ScienceDirect
Materials Science & Engineering A
0921-5093/$ - see front matter&2012 Elsevier B.V. All rights reserved. http://dx.doi.org/10.1016/j.msea.2012.11.095
Corresponding author. Tel.:þ44 1895 266663; fax:þ44 1895 269758.
agreement in the most popular Al–Si cast alloys, but it is inconsistencies for the inﬂuence of Fe on the mechanical proper-ties of castings . Meanwhile, the amount of Mn needed to neutralize Fe has not been well established[19,20]. Although Mn/ Fe ratio of 0.5 is desirable for the transformation of
The formation of Fe-rich intermetallics is greatly affected by solidiﬁcation conditions during casting[21,22]. The superheat and cooling rate have been reported to affect the nucleation and growth of the Fe-rich phases and thus to be able to modify the morphology and size of the intermetallics in aluminium alloys[23,24]. At high cooling rates as in the case of HPDC, the occurrence of primary
b-AlFeSi needles is shifted towards higher iron levels at Fe41% [25,26]. These observations are important in understanding the microstructure features of Al–Si and Al–Si–Cu cast alloys. However, insight in solidiﬁcation of other alloys is still limited in terms of the Fe-rich intermetallic phases at different contents of Fe and Mn, especially under high cooling rate with HPDC process. Meanwhile, the thermodynamic modelling by CALPHAD is becoming an impor-tant tool in alloy development, which can determine the phase formation under the equilibrium condition. The thermodynamic modelling of Al–Fe–Mn–Si system has been carried out by Balitchev et al.. They achieved reasonably good results by treating the
a-AlFeMnSi phase as a stoichiometric compound. The similar approaches were also used by Fang et al.for the formation of Fe-rich intermetallics in semisolid processed A380 and A356 alloys. These results provided a guideline for understanding the solidiﬁca-tion and phase formasolidiﬁca-tion process. Therefore, the further investiga-tion for the phase formainvestiga-tion of Fe-rich intermetallics in the diecast Al–Mg–Si (–Mn) alloys is necessary in order to enhance the under-standing towards the integration of thermodynamics, solidiﬁcation and microstructural evolution, and mechanical properties. This is practically important in materials recycling where the various elements and the different amount of corrector elements are required during casting.
The present study attempts to investigate the effect of Mn and Fe on the morphology, size and distribution of various Fe-rich com-pounds in the Al–Mg–Si alloy produced by HPDC process. The mechanical properties of yield strength, ultimate tensile strength and elongation were assessed with different Fe and Mn contents. The role of alloy chemistry on the effect of Fe and Mn was investigated by CALPHAD modelling of multi-component Al–Mg– Si–Mn–Fe and Al–Mg–Si–Fe systems. The thermodynamic model-ling and the experimental ﬁndings of the Fe-rich intermetallic compounds were studied with respect to the role of Mn on combating the detrimental effect of Fe in the Al–Mg–Si alloy. The discussions are focused on the phase formation of different Fe-rich intermetallic phases and the relationship between Fe-rich com-pounds and mechanical properties of the diecast Al–Mg–Si alloys.
The Al–Mg–Si alloys with different Fe and Mn contents were produced by melting the ingots of commercial pure aluminium, pure
magnesium and the master alloys of Al-15 wt%Si, Al-20 wt%Mn, Al-10 wt%Ti and Al-80 wt%Fe. During the experiments, each element was weighed to a speciﬁed ratio with different extra amounts for burning loss compensation during melting. The 6–10 kg melt was prepared in a clay-graphite crucible using an electric resistance furnace. The processing temperature of the melt ranged between 690 and 7501C. For all the experiments, the melt was subjected to
ﬂuxing and degassing using commercial ﬂuxes and N2. The N2 degassing usually lasted 3 min and the granular ﬂux covered on the top surface of the melt during N2 degassing. The sample for composition analysis was taken from the melt after homogenisation. A
f4060 mm cylindrical sample was made by casting the melt directly into a steel mould for the composition analysis. The casting was cut across the diameter at 15 mm from the bottom and ground down to 800 grid abrasive grinding paper. The composition of each alloy was obtained from an optical mass spectroscopy, in which at least ﬁve spark analyses were per-formed and the average value was taken as the chemical compo-sition of alloy. The compocompo-sition was further conﬁrmed by area energy dispersive X-ray (EDX) quantiﬁcation in SEM. The actual compositions of the alloys containing 0.02 wt% and 0.54 wt% Mn are shown inTable 1.
Compositions of diecast Al–Mg–Si alloys used in experiments (wt%).
Alloy Si Fe Mn Mg Ti Zn Others Al A 2.270.08 variedn 0.54170.05 6.270.08 0.1770.04 0.01270.004 o0.03 Bal. B 1.970.07 varieda 0.02370.04 5.670.09 0.1570.04 0.01370.004 o0.03 Bal. n
Actual Fe contents were measured to be 0.214, 0.389, 0.623, 0.841, 1.243, 1.490, 1.861, and 2.482, respectively. a
Actual Fe contents were measured to be 0.086, 0.414, 0.634, 0.911, 1.188, 1.420, 1.542, and 1.821, 2.453, respectively.
Fig. 1.Diagram of die castings for the standard tensile testing samples of cast
aluminium alloy according to the speciﬁcation deﬁned in ASTM B557-06. The overﬂow and biscuit are designed in associated with cold chamber die casting machine. The dimensions are in mm.
After composition analysis and skimming, the melt was manually dosed and subsequently released into the shot sleeve of a 4500 kN HPDC machine for the ﬁnal casting, in which all casting parameters were fully monitored. The pouring tempera-ture was measured by a K-type thermocouple, usually at 501C
above the liquidus of the alloy according to the equilibrium phase diagram. Six ASTM standard samples with three
f6.35 mm round bar and three square bar were cast in each shot. The diagram of die castings for the standard tensile testing samples is shown in
Fig. 1. The casting die was heated by the circulation of oil at 2501C. All castings were kept at ambient condition for at least
24 h before the mechanical property test.
The tensile tests were conducted following the ASTM B557 standard using an Instron 5500 Universal Electromechanical Testing Systems equipped with Bluehill software and a750 kN load cell. All the tests were performed at ambient temperature (251C). The gauge length of the extensometer was 25 mm and
the ramp rate for extension was 2 mm/min. Each data reported is
α1 α1 α2 α2 α2 α1 α1 α2 α2 α1 α1 α2 α1 α1 α2 α2
Fig. 2.Optical micrographs showing the microstructure of diecast alloy with different amounts of Fe and Mn, (a) 0.54Mn, 0.21Fe, (b) 0.02Mn, 0.09Fe, (c) 0.54Mn, 0.62Fe,
based on the properties obtained from 10 to 30 samples without showing obvious casting defects on the fractured surfaces.
The specimens for microstructure examination were cut from the middle of
f6.35 mm round tensile test bars. The microstruc-ture was examined using a Zeiss optical microscopy with quanti-tative metallography, and a Zeiss SUPRA 35VP scanning electron microscope (SEM), equipped with EDX. The particle size, volume fraction and the shape factor of the solid phase were measured using an AxioVision 4.3 Quantimet digital image analysis system. The quantitative EDX analysis in SEM was performed at an accelerating voltage of 20 kV on a polished sample, and the libraries of standard X-ray proﬁles for EDX were generated using pure elements. In situ spectroscopy calibration was performed in each session of the EDX quantiﬁcation using pure copper. To minimise the inﬂuence from the interaction volume during the EDX quantiﬁcation, ﬁve point analyses on selected particles were conducted for each phase and the average was taken as the measurement.
3.1. As-cast microstructure of the diecast Al–Mg–Si alloys
In the as-cast state, there was no signiﬁcant change in the morphologies of the primary
a-Al phase and eutectic phase presented in the Al–Mg–Si alloys containing different levels of Fe and Mn. However, the primary
a-Al solid solution was found in two types of morphology in each alloy, which are labelled as ‘
a1’ and ‘
a2’ inFig. 2, respectively. The
a1-Al phase was formed in the shot sleeve, in which the cooling rate is up to 102K/s during solidiﬁcation. This resulted in the formation of dendrites and fragmented dendrites in the microstructure. The
a2-Al phase was believed to be formed in the die cavity under a cooling rate over 103K/s during solidiﬁcation, which showed ﬁne globular mor-phology in the microstructure. The sizes of dendritic and frag-mented dendritic
a1-Al phase ranged from 20 to 100
mm and the ﬁne globular
a2-Al particles ranged from 3 to 20
mm. The coarse
a1-Al phase was isolated by ﬁne globular
a2-Al particles. The interdendritic regions were characterised with a eutectic micro-structure (labelled as ‘E’ inFig. 3), in which the lamellar structure was made of
a-Al and Mg2Si phases. The primary
a-Al phase was associated with the eutectic microstructure. Fe-rich intermetallic compounds were observed in the eutectic areas. In order to simplifying the explanation, the solidiﬁcation in the shot sleeve is described as ﬁrst solidiﬁcation and the solidiﬁcation in the die cavity is described as secondary solidiﬁcation.
In contrast to the primary
a-Al phase, it is seen that the effect of Fe and Mn on the morphologies of primary Fe-rich compounds was signiﬁcant. Different types and amounts of the Fe-rich intermetallics were related to the Fe and Mn contents, as shown inFigs. 2 and 4. From the experimental observations, only a small amount of ﬁne intermetallic compounds were present in the alloys that contain up to 0.21 wt%Fe (Figs. 2 and 4a and b). The ﬁne Fe-rich intermetallics were formed in the secondary solidiﬁ-cation inside the die cavity (labelled as ‘Fe2’ inFig. 4). Most of the ﬁne intermetallics were located between the primary
a-Al phase (
a2-Al), although some intermetallics were found inside them. No primary Fe-rich intermetallic compounds were observed in the primary
a-Al phase precipitated in the ﬁrst solidiﬁcation. The EDX quantitive analysis by SEM identiﬁed the Fe-rich phase with the typical composition of the
a-Al24 (Fe,Mn)6Si2phase in the Al–Mg–Si alloy with Mn addition and the
a-Al8Fe2Si phase in the Al–Mg–Si alloy without Mn addition. No
b-AlFeSi intermetallics were observed in the samples at this composition.
When the Fe contents in the alloys were increased to a level of 1.2 wt%Fe, there were two types of Fe-rich intermetallics observed. In the Al–Mg–Si alloy with Mn addition (Fig. 4c and d, e and f), the Fe-rich intermetallics were formed in both the ﬁrst solidiﬁcation and the secondary solidiﬁcation, which were labelled as ‘Fe1’ and ‘Fe2’, respectively. The Fe1-rich intermetallics were usually associated with the primary
a1-Al phase and exhibited coarse compact morphology, which were found in tetragonal, pentagonal, hexagonal shapes. EDX quantiﬁcation has identiﬁed the Fe-rich intermetallics to be the
a-AlFeMnSi phase with the typical composition of
a-Al24(Fe,Mn)6Si2. Mean-while, the ﬁne intermetallics (labelled as Fe2) were associated with
a2-Al phase and segregated in the primary
a-Al grain boundaries, which were identiﬁed by EDX quantiﬁcation to be the same
a-AlFeMnSi phase with the typical composition of
a-Al24(Fe,Mn)6Si2. In the Al–Mg–Si alloy without Mn addition (Fig. 4d and f), the ﬁne Fe-rich phase was also found at the primary
a-Al grain boundaries, which exhibited similar morphol-ogy and size to that in the alloy with Mn addition. The ﬁne Fe-rich intermetallic phase was identiﬁed as the
a-AlFeSi phase with the typical composition of
a-Al8Fe2Si. However, the primary Fe-rich phase formed in the ﬁrst solidiﬁcation showed very different morphology in comparison with that formed in the alloy with Mn addition. As seen in Fig. 4d and f, the Fe1-rich phase exhibited needle-shaped morphology, which crossed through both the primary
a-Al phases formed in the ﬁrst solidiﬁcation and the secondary solidiﬁcation. The EDX quantiﬁcation conﬁrmed that the needle-shaped Fe-rich phase was
b-AlFe phase with the typical composition of
b-Al13Fe4. It is clearly seen that the additions of Mn can extent the range of Fe contents to form
a-AlFeMnSi phase in the alloys. In other words, the Fe content to initialize the
b-AlFe phase is increased by adding Mn in the alloys. When the Fe contents in the alloys was further increased to a level of 1.8 wt% in Al–Mg–Si–Mn–Fe and Al–Mg–Si–Fe systems. In the Al–Mg–Si alloy with Mn addition, as shown inFig. 4g, a large fraction of long needle-shaped Fe-rich intermetallics were found in the microstructure (bright strip inFig. 4g), in addition to the compact Fe-rich phase. The coarse and the ﬁne compact primary Fe-rich intermetallics were identiﬁed by EDX quantiﬁcation as the
a-AlFeMnSi phase with the typical formula of
a-Al24(Fe,Mn)6Si2. The long needle-shaped Fe-rich compounds were quantitively
Fig. 3.SEM micrograph showing the typical microstructure of eutectic Al–Mg2Si
b-AlFe phase with the typical composition of
b-Al13(Fe,Mn)4Si0.25. In the alloy without Mn addition, as shown in Fig. 4h, a large fraction of the long needle-shaped primary Fe-rich intermetallics were found in the microstructure, which were conﬁrmed by EDX as
b-AlFe phase with the typical compo-sition of
b-Al13Fe4. Only a small fraction of Fe-rich intermetallic compounds were in the form of compact format, which was conﬁrmed by EDX as
a-AlFeSi phase with the typical composition of
In the as-cast microstructure, some coarse Fe-rich intermetallics developed into more complex morphologies such as star-like shapes in associated with primary
a-Al phase, as shown in Fig. 5. These Fe-rich intermetallics have been found in the castings with experi-mental composition of Fe40.6 wt % and identiﬁed as
a-AlFeMnSi phase with the typical composition of
a-Al24(Fe,Mn)6Si2. It was also found that the star-like
a-AlFeMnSi phase were usually associated with
a1-Al phase formed in the shot sleeve. The results indicate that the solidiﬁcation environments, especially the cooling rate in the
5µm 5µm 5µm 5µm 5µm 5µm 5µm 5µm Fe2 α1-Al α2-Al α1-Al α2-Al Fe2 Fe1 Fe2 α1-Al α2-Al Fe2 Fe1 α1-Al α2-Al Fe2 Fe1 α1-Al α2-Al α1-Al α2-Al
Fe2 Fe1 α2-Al Fe2 Fe1 Fe1 Fe1 α2-Al α1-Al Fe2
Fig. 4.Backscattered SEM micrographs showing the morphology of Fe-rich intermetallics in the diecast alloy with different amounts of Fe and Mn, (a) 0.54Mn, 0.21Fe,
shot sleeve is capable of producing different morphologies of primary
From these observations, the Fe-rich compounds of the com-pact and needle-shaped morphologies were identiﬁed as the
b-AlFe phase, respectively. The inter-metallic compounds in the Al–Mg–Si alloys with and without Mn addition are summarised inTable 2. It is seen that the primary
a-Al24(Fe,Mn)6Si2 intermetallics formed in the die cavity were observed in all diecast alloys in the experimental range. However, the primary Fe-rich intermetallics formed in the shot sleeve were signiﬁcantly affected by the Fe contents. It is noticeable that the intermetallic
b-Al13Fe4phases formed in the experimental alloys were different to the intermetallic
b-AlFeSi phases observed in Al–Si, Al–Si–Cu and Al–Si–Mg alloys[9,18,20]. However, the cubic
a-AlFeMnSi phase of
a-Al24(Fe,Mn)6Si2 intermetallics formed in the experimental alloys was found to be very similar to
a-Al15(FeMn)3Si2 inter-metallics formed in Al–Si, Al–Si–Cu and Al–Si–Mg alloys[6,16,28]. In order to characterize the Fe-rich intermetallics in the alloys, their sizes and solid fractions were measured in the microstruc-ture. The results for the ﬁne
a-AlFeMnSi and ﬁne
a-AlFeSi particles that are formed in the die cavity are shown inFig. 6. Both particles followed a level correspondence to the Fe contents, which were consistently at 0.76
mm in diameter and no signiﬁ-cant variation within the experimental ranges (Fig. 6a). The distribution of the ﬁne Fe-rich particles was well matched by the normal distribution curve with an average of 0.76 (Fig. 6b). However, the volume fraction of the ﬁne Fe-rich particles increased with the increase of Fe contents in the alloys (Fig. 6c). As the ﬁne Fe-rich particles were formed during the solidiﬁcation in the die cavity under high cooling rate, the results indicate that
the sizes of the Fe-rich intermetallics were mainly determined by the increased undercooling, enhanced heterogeneous nucleation and the shortened solidiﬁcation time for the particle to grow.
In the Al–Mg–Si alloys with and without Mn addition, it is seen that the average sizes and volume fractions of the Fe-rich intermetallics solidiﬁed in the shot sleeve were obviously differ-ent to that formed in the die cavity, as shown in Fig. 7. The volume fraction and the size of the primary Fe-rich intermetallics 20μm
Fig. 5.Backscattered SEM micrograph showing the morphology of Fe-rich
inter-metallics in the diecast Al–5Mg–2Si alloy with 0.54Mn and 0.84Fe.
Average compositions of Fe-rich intermetallic phases measured by quantitive SEM/EDX analysis. Mn (wt.%) Phase morphology Identiﬁed compounds Al Fe Mn at% Si Fe/ Mn 0.54 Coarse compact Al24(Fe,Mn)6Si2 76.64 11.83 5.95 6.27 1.99 Fine compact Al24(Fe,Mn)6Si2a 75.47 12.16 6.28 6.09 1.94 Large needle Al13(Fe,Mn)4Si0.25 75.62 19.20 3.81 1.37 5.04 0.02 Fine compact Al8Fe2Sia 35.01 9.59 – 4.13 –
Large needle Al13Fe4 75.50 24.51 – – – a
The composition was further conﬁrmed by TEM/EDX analysis.
0.0 0.5 1.0 1.5 2.0 0.0 0.5 1.0 1.5 2.0 A v
erage particle size (
μ m) 0.54Mn 0.02Mn 0 4 8 12 16 20 0.0 0.4 0.8 1.2 1.6 2.0 Frequency (%) Particle size (μm) 0.54Mn 0.02Mn 0 1 2 3 4 0 0.5 1 1.5 2 Solid fraction of Fe Fe (wt.%) Fe (wt.%) 0.54Mn 0.02Mn
Fig. 6.Effect Fe contents in the diecast alloy on (a) the average size, (b) the
frequency and (c) the volume fraction of Fe-rich intermetallic phase solidiﬁed in the die cavity.
increased signiﬁcantly with the increase of Fe contents in the alloys. However, the size of the Fe-rich intermetallics increased in different ways. A linear increase of the size in the Fe-rich intermetallics was found in the alloys without Mn addition, but the size of Fe-rich intermetallics followed two separate linear correspondences to the Fe contents at a vertex of 1.24 in the alloy with Mn addition. A gradual increase was found at Feo1.24 wt% and a signiﬁcant increase was found at Fe41.24 wt%. The vertex in Fig. 7b conﬁrmed that the critical Mn/Fe ratio is at level of 0.5 to suppress the formation of
b-Al13(Fe,Mn)4Si0.25in the alloys. 3.2. Mechanical properties
Mechanical properties of the diecast Al–Mg–Si alloys with different Fe and Mn contents are presented inFig. 8. It is seen that a slight enhancement in the yield strength and a signiﬁcant detrimental to the elongation with the increase of Fe contents in the alloys. However, no obvious variation in the ultimate tensile strength was observed until Fe was higher than 0.6 wt% where it decreased. Overall, the strength and the elongation of the diecast alloys with different Fe levels were all effectively higher in the alloys with 0.54 wt%Mn than these of their diecast counter-parts with 0.02 wt%Mn. In addition to the slightly variation of Mg and Si concentrations in the alloys, as shown inTable 1, the
difference in Mn content was one of the major factors to affect the strength and elongation of the diecast alloys. It is worth for a further emphasis that the enhancement of the yield strength for the diecast samples is less effective than the detrimental to the elongation of the same alloy in the experimental ranges.
0 5 10 15 20 0 0.5 1 1.5 2 Solid fraction of Fe Fe (wt.%) 0.54Mn 0.02Mn 0 20 40 60 80 100 0.0 0.5 1.0 1.5 2.0 Size (μm) Fe (wt.%) 0.54Mn 0.02Mn
Fig. 7.Effect of Fe contents in the diecast alloy on (a) the volume fraction and
(b) the average size of Fe-rich intermetallic phase solidiﬁed in the shot sleeve.
40 80 120 160 200 0 0.5 1 1.5 2 2.5 Y
ield strength (MPa)
Fe (wt.%) 0.02Mn 0.54Mn 200 250 300 350 0 0.5 1 1.5 2 2.5
Ultimate tensile strength (MPa)
Fe (wt.%) 0.02Mn 0.54Mn 0 5 10 15 20 25 0 0.5 1 1.5 2 2.5 Elongation (%) Fe (wt.%) 0.02Mn 0.54Mn
Fig. 8.Effect of Fe content on the mechanical properties of die cast Al–Mg–Si
alloys with different amounts of Mn, (a) yield strength, (b) ultimate tensile strength, and (c) elongation.
The overall increase of the yield strength of the diecast sample was 8% while the ultimate tensile strength decreased by 9% and the elongation decreased by 295%.
3.3. CALPHAD of the multi-component Al–Mg–Si–Mn–Fe and Al–Mg–Si–Fe systems
In order to understand the effect of alloying on solidiﬁcation and microstructural evolution, CALPHAD modelling of the multi-component Al–Mg–Si–Mn–Fe and Al–Mg–Si–Fe systems was carried out using PandaT software . The Ti and other low levels of elements were not considered. The COST507 thermo-dynamic database  was used for constituent alloy systems and the
a-AlFeMnSi was treated as a stoichiometric phase during the modelling. The calculated equilibrium phase diagrams on the cross sections of Al–5Mg–2Si–0.5Mn–xFe and Al–5Mg–2Si–xFe are shown inFigs. 9 and 10, respectively.
For the Al–Mg–Si–Mn–Fe system, the calculated diagram shown inFig. 9can be divided into several regions with different Fe contents. The phase formation follows: (1) L-
MnSiþMg2Si with prior
a-Al phase at Feo(0.25 wt%), and (2) L
a-AlþMg2Si with prior
a-AlFeMnSi phase at 0.21 wt%oFeo1.4 wt%, and (3) L-
Mg2Si with prior
b-AlFe phase at Fe41.4 wt%. It needs to emphasise that the
b-AlFe phase can be formed with a very low Fe content according the equilibrium phase diagram. However, the formation of
b-AlFe phase in the as-cast microstructure of the experimental alloys with 0.54 wt%Mn is from 1.2 wt%Fe. The difference may be attributed to several factors including the noon-equilibrium solidiﬁcation in HPDC process, the complex of precipitation process of intermetallics during solidiﬁcation, and the database used in phase diagram calculation.
Similarly, for the Al–Mg–Si–Fe system shown inFig. 10, the solidiﬁcation procedure roughly follows: (1) L-
a-AlFe-SiþMg2Si with prior
a-Al phase at Feo(0.98 wt%), in which
b-AlFe phase may exist at 0.22 wt%oFeo0.98 wt%, and (2) L
a-AlþMg2Si with prior
b-AlFe phase at Fe40.98 wt%. The experimental results should that the
b-AlFe phase was observed in the alloy with Fe content higher than 0.62 wt%.
The effect of Mn and Fe contents on the formation of Fe-rich intermetallic compounds are further demonstrated inFig. 11for the Al–Mg–Si alloys with three different levels of Mn contents at 0.2, 0.4 and 0.6 wt%, respectively. It is seen that the Fe content was lowered to form prior
a-Al phase with the increases of Mn contents in the alloy. In other words, with the increase of Mn in the alloy, the
a-AlFeMnSi was formed as prior phase at a lower level of Fe content in the alloy. Meanwhile, the addition of Mn also increased the Fe levels to form
b-AlFe phase. Therefore, the area to form
a-AlFeMnSi was signiﬁcantly enlarged with the increase of Mn contents. This implies that the addition of Mn in the alloy can suppress the formation of
b-AlFe intermetallic compounds in the alloy with practically possible high Fe content. On the other side, as seen inFig. 11, the results conﬁrmed that the increase of Mn in the alloy resulted in a signiﬁcant increase of liquidus temperature of the alloy.
4.1. Phase formation in diecast Al–Mg–Si alloy
The experimental observations have conﬁrmed that (1)
a-AlFeMnSi intermetallics can be formed in two solidiﬁcation stages
0 1 2 3 600 650 700 550 Fe (wt.%) Temperature (wt.%) Liquid αAl+Mg2Si + αAlFeMnSi L + βAlFe L + βAlFe+ αAlFeMnSi L + αAlFeMnSi
L + βAlFe+ αAlFeMnSi + αAl
βAlFe+ αAlFeMnSi + αAl +Mg2Si L + αAl L + αAl +αAlFeMnSi 0.5 1.5 2.5 0.25 1.40 1.30 0.85 1.11 0.92
Fig. 9.Cross section of equilibrium phase diagram of Al–5Mg–2Si–0.6Mn–xFe
calculated by Pandat software.
700 670 640 610 580 550 0 0.5 1.0 1.5 2.0 2.5 3.0 L + βAlFe L + βAlFe + αAl L L + αAl L + αAl + αAlFeSi L + βAlFe + αAl + αAlFeSi βAlFe + αAl + αAlFeSi+Mg2Si αAl + αAlFeSi +Mg2Si T e mperature ( οC) 0.22 0.98 1.68 2.37 1.31 0.33 Fe (wt.%)
Fig. 10.Cross section of equilibrium phase diagram of Al–5Mg–2Si–xFe calculated
by Pandat software. 0 1 2 3 4 620 660 700 680 640 600 Fe (wt.%) Temperature ( οC) L+ βAlFe α-Al L 0.2wt.%Mn 0.4wt.%Mn 0.6wt.%Mn
Fig. 11.Effect of Mn on the cross section of equilibrium phase diagram of
during HPDC, one is in the shot sleeve and the other is in the die cavity, which show the compact morphology with different sizes; (2) manganese increases the Fe content range over which
a-AlFeMnSi phase forms; (3) the Mn/Fe ratio at 0.5 is applicable to form
b-AlFe intermetallics in the Al–Mg–Si–Mn alloy during HPDC; (4) no
b-AlFeSi intermetallics are observed in the Al–Mg–Si diecast alloys with varied Mn and Fe contents.
Generally, the phase formation of Fe-rich intermetallics in the experimental alloys is broadly consistent with the equilibrium phase diagram calculated from CALPHAD. Therefore the solidiﬁ-cation path can be used to explain the major features of the microstructure. The solidiﬁcation process and the associated changes of liquid compositions determine the formation of different phases. From the phase diagram inFig. 9, it is seen that the prior phase is
a-Al phase when Fe content is less than 0.25 wt%. The solidiﬁcation starts to precipitate the
a-Al phase in the shot sleeve, which is interrupted during die ﬁlling. The precipitation of
a-Al phase continues in the die cavity, during which Si, Fe and Mn elements are enriched in the remaining liquid and the Fe-rich intermetallics are consequently formed in the melt. The high cooling rate in the die cavity and the absence of superheat in the melt enhance the heterogeneous nucleation, and therefore promote the formation of ﬁne compact
a-AlFeMnSi intermetallics. When Fe content is increased to a higher level, the prior phase becomes
a-AlFeMnSi. The precipitation of
a-AlFeMnSi compounds increases the undercooling in front of the interface of the crystal, resulting in the nucleation and growth of
a-Al phase in associated with
a-AlFeMnSi compounds (Figs. 2 and 4). The solidiﬁcation continues in the die cavity,
where the compact
a-AlFeMnSi compounds and
precipitate under high cooling rate. When Fe content is further increased, the prior phase is
b-AlFe phase. The precipitation of
b-AlFe compounds consumes Fe element in the melt and thus alters the local melt composition with enriched Si and Mn, resulting in an increase of Mn/Fe ratio. When Mn/Fe ratio reaches the limitation,
a-AlFeMnSi compound precipitates from the melt. The following solidiﬁcation precipitate the
b-AlFe compounds. Overall, the formation of
b-AlFe phases consumes Fe, Mn, Si prior to the eutectic solidiﬁca-tion. The ﬁnal stage of solidiﬁcation of the alloys is the multi-eutectic transformation to generate the multi-eutectic structure mainly of Al–Mg2Si eutectic phase.
Mn is largely consumed by the formation of the Fe-rich intermetallics. Therefore, an adequate level of Mn is necessary in order to maintain high Mn/Fe ratio for the formation of the cubic
a-AlFeMnSi phase. In the observed
a-AlFeMnSi intermetal-lics, the typical composition is
a-Al24(Fe,Mn)6Si2, which is made of less Si than that in the common
a-Al15(FeMn)3Si2compounds. The main reason can be attributed to the low Si concentration in the alloy and the short of Si supply during solidiﬁcation. In the experimental results, it is also conﬁrmed that Mn/Fe¼0.5 is necessary to suppress the formation of the
b-AlFe compounds in the as-cast microstructure.
b-AlFe intermetallics is immediately observed in the alloys when Mn/Feo0.5, which is in good agreement with the observation in other alloys including Al–Si, Al–Si–Cu and Al–Si–Mg alloys [6–13]. However,
a-AlFeMnSi phase can still be observed at low Mn/Fe ratio. Therefore, the Mn/Fe ratio can be used as an indicator for the formation of
b-AlFe compounds, but not for determining the formation of
The absence of
b-Al5FeSi intermetallics in the diecast Al–Mg– Si alloy is one important feature. In the equilibrium state, the
b-Al5FeSi intermetallics has a monoclinic crystal structure with the lattice parameters a¼b¼0.612 nm,c¼4.15 nm, and
b¼911 ora¼b¼0.618 nm,c¼4.15 nm, and
b¼911. Similarly, the
crystal structure of
b-Al13Fe4phase is also monoclinic
with a¼1.549 nm, b¼0.808 nm, c¼1.248 nm,
Currently, it is still not clear for the conditions to form
b-Al13Fe4) in Al alloys. The effect factors are suspected in associated with the content of Fe and Si, in which low Fe contents and high Si/Fe ratio favour the formation of
b-Al5FeSi phase, but high Fe contents and low Si/Fe ratio tend to form
b-Al3Fe (Al13Fe4) phase. Obviously, the more systematic work needs to address the mechanism in future.
4.2. Microstructure-property relationship
The experimental results have conﬁrmed that the Fe-rich intermetallics signiﬁcantly affect the mechanical properties of the Al–Mg–Si alloys. The higher the iron concentrations in the alloy, the signiﬁcantly more the elongation decreases. This is accompanied by a slight enhancement of the yield strength at increased iron level in the alloys. The ultimate tensile strength maintains at similar level when Fe is less than 0.6 wt%, but it decreases signiﬁcantly when the Fe contents further increases. Meanwhile, a slight enhancement of the yield strength is also observed in the alloy with Mn addition compare to that in the alloy without Mn addition.
Referring to the solidiﬁcation microstructure, the enhanced yield strength is believed to correspond to the increased amounts of Fe-rich intermetallic compounds, especially the ﬁne interme-tallics present at the
a-Al grain boundaries. The increase in yield strength is accompanied with decreasing elongation as the added reinforcement due to the Fe-rich compounds is at the cost of the alloy ductility. Therefore the detrimental effect of iron content on the mechanical properties in the diecast Al–Mg–Si alloys should be determined mainly by the loss in ductility.
Mn introduces an overall superiority in the elongation largely due to its effective role on modifying the morphologies and sizes of the primary Fe-rich intermetallic compounds. Long-needle shaped
b-AlFe is either eliminated or modiﬁed into less harmful compact
a-AlFeMnSi intermetallics by the Mn addition. Therefore, the elongation of the alloy with Mn addition is higher than that of their counterparts without Mn addition. However, the improvement of ductility vanishes in the alloys when Fe41.2 wt%, where large
b-AlFe needles precipitate in the microstructure.
1) In high pressure die casting of Al–Mg–Si–(Mn) alloys, the formation of Fe-rich intermetallics occurs into two solidiﬁca-tion stages. One is in the shot sleeve at lower cooling rates, and the other is in the die cavity at higher cooling rates. The Fe-rich intermetallics formed in the shot sleeve exhibit coarse com-pact, star-like or needle/plate shape morphology with varied sizes. The Fe-rich intermetallics formed in the die cavity are characterised by ﬁne compact morphology with the size less than 3
2) In diecast Al–Mg–Si alloys, two types of Fe-rich intermetallics are formed over the Fe content range up to 2.4 wt %. The ﬁne compact
a-AlFeSi phase has the composition of
a-Al8Fe2Si and the long needle
b-AlFe phase has the composition of
b-Al13Fe4. With 0.54 wt%Mn being added into the alloy, the ﬁne compact intermetallic phase is found to be Al24(Fe,Mn)6Si2and the long needle
b-AlFe phase is
3) In diecast Al–Mg–Si alloys containing 0.54 wt%Mn, the prior phase is
a-Al when Fe is less than 0.21 wt%, but the prior phase is
b-Al13(Fe,Mn)4Si0.25 when Fe is higher than 1.24 wt%. Over the Fe contents range from 0.21 to 1.24 wt%,
a-Al24(Fe,Mn)6Si2 precipitates as prior phase to form either coarse compact
compounds in the shot sleeve or ﬁne compact particles in the die cavity.
4) The morphology and size of
a-Al24(Fe,Mn)6Si2 intermetallics are dependent on the cooling rate. The higher cooling rate in the die cavity enables the
a-Al24(Fe,Mn)6Si2phase to solidify in a ﬁne compact morphology. However, the lower cooling rate in the shot sleeve results in the formation of compact and star-like Chinese script
a-Al24(Fe,Mn)6Si2 phase in the as-cast microstructure.
5) Fe-rich intermetallics signiﬁcantly affect the mechanical prop-erties of the alloy castings. The higher the iron concentrations in the alloy, the more signiﬁcantly the ductility reduces. This is accompanied by a slight enhancement of the yield strength. The ultimate tensile strength maintains the similar level when Fe contents is less than 0.6 wt%, but decreases signiﬁcantly with the further increase of Fe contents in the diecast alloys. 6) The yield strength and the ultimate tensile strength are
slightly enhanced in the diecast Al–Mg–Si alloy when Mn is added in comparison with that without Mn addition.
7) Manganese promotes the formation of the cubic
a-AlFeMnSi phase and suppresses the formation of
b-AlFe phase in diecast Al–Mg–Si alloys. The
b-AlFe compounds are formed when Mn/Fe ratio is less than 0.5.
The authors acknowledge the EPSRC and JLR for ﬁnancial support.
 S. Ji, D. Watson, Z. Fan, M. White, Mater. Sci. Eng., A 556 (2012) 824–833.  L. Wang, M. Makhlouf, D. Apelian, Int. Mater. Rev. 40 (1995) 221–238.  J.L. Jorstad, Die Cast. Eng. (1986) 30–36. (Nov/Dec.
 Z. Yi, Y.X. Gao, P.D. Lee, T.C. Lindley, Mater. Sci. Eng., A 386 (2004) 396–407.  G.B. Winkelman, Z.W. Chen, D.H. StJohn, M.Z. Jahedi, J. Mater. Sci. 39 (2004)
 P. Skjerpe, Metall. Mater. Trans. A 18A (1987) 189–200.
 L.F. Mondolfo, Aluminium Alloys: Structure and Properties, Butterworth, London, 1976 534.
 L. Backerud, G. Chai, J. Tamminen, Solidiﬁcation Characteristics of Aluminium Alloys, Foundry Alloys 2 (1990) 71–84. (AFS/Skanaluminum.
 S. Shivkumar, L. Wang, D. Apelian, JOM 43 (1991) 26–32.
 M.V. Kral, H.R. McIntyre, M.J. Smillie, Scr. Mater. 51 (2004) 215–219.  J.G. Zheng, R. Vincent, J.W. Steeds, Philos. Mag. 79 (1999) 2725–2733.  K.Y. Wen, W. Hu, G. Gottstein, Mater. Sci. Technol. 19 (2003) 762–768.  A. Couture, AFS Int. Cast. Met. J. 6 (1981) 9–17.
 P.N. Crepeau, AFS Trans. 103 (1995) 361–366.  D. Munson, J. Inst. Met. 95 (1967) 217–219.
 P. Hodgson, B.A. Parker, J. Mater. Sci. 16 (1981) 1343–1348.
 S.G. Shabestari, J.E. Gruzleski, Metall. Mater. Trans. 26A (1995) 999–1006.  X. Cao, J. Campbell, Int. J. Cast Met. Res. 13 (2000) 175–184.
 C. Mascre, Fonderie 108 (1995) 4330–4336.
 X. Cao, J. Campbell, Metall. Mater. Trans. A 35A (2004) 1425–1435.  G.K. Sigworth, S. Shivkumar, D. Apelian, AFS Trans. 97 (1989) 811–824.  A. Pennors, A.M. Samuel, F.H. Samuel, H.W. Doty, AFS Trans. 106 (1998)
 L.A. Narayanan, F.H. Samuel, J.E. Gruzleski, Metall. Mater. Trans. A 25A (1994) 1761–1773.
 S. Seifeddine, I.L. Svensson, Metall. Sci. Technol. (2009) 11–20 27-1-Ed.  A.M. Samuel, A. Pennors, C. Villeneuve, F.H. Samuel, Int. J. Cast. Met. Res. 13
 X.P. Niu, B.H. Hu, S.W. Hao, J. Mater. Sci. Lett. 17 (1998) 1727–1729.  E. Balitchev, T. Jantzen, I. Hurtado, D. Neusch ¨utz, Calphad 27 (2003) 275–278.  X. Fang, G. Shao, Y.Q. Liu, Z. Fan, Mater. Sci. Eng. A 445–446 (2007) 65–72.  S.-L. Chen, S. Daniel, F. Zhang, Y.A. Chang, X.-Y. Yan, F.-Y. Xie, R.
Schmid-Fetzef, W.A. Oatesd, Calphad 26 (2002) 175–188.
 I. Ansara, A.T. Dinsdale, M.H. Rand (Eds.), COST 507-Final Report: Thermo-dynamic Database for Light Metal Al-alloys, vol.2, European Communities, Brussels, 1998.
 R. Høier, O. Lohne, S. Mørtvedt, Scand. J. Metall. 6 (1977) 36–37.  P. Skjerpe, J. Microsc. 148 (1987) 33–50.
 L. Sweet, S.M. Zhu, S.X. Gao, J.A. Taylor, M.A. Easton, Metall. Mater. Trans. A 42A (2011) 1737–1749.